- Nano Express
- Open Access
Monolayer Phosphorene–Carbon Nanotube Heterostructures for Photocatalysis: Analysis by Density Functional Theory
Nanoscale Research Letters volume 14, Article number: 233 (2019)
One-dimensional (1D)/2D heterostructures have attracted great attention in electronic and optoelectronic fields because of their unique geometrical structures and rich physics. Here, we systematically explore electronic structure and optical performance of single-wall carbon nanotube (CNT)/phosphorene (BP) hybrids by large-scale density functional theory (DFT) computation. The results show that the interfacial interaction between CNT and BP is a weak van der Waals (vdW) force and correlates with tube diameter of CNTs. The CNT/BP hybrids have strong optical absorption compared with that of individual BP and CNT. A diameter-dependent type I or II heterojunction in CNT/BP hybrids is observed. Moreover, CNTs can not only significantly promote photogenerated carrier transfer, but also effectively improve the photocatalytic activities of BP as a co-catalyst. These findings would enrich our understanding of BP-based 1D/2D heterostructures, providing further insight into the design of highly efficient phosphorene-based or CNT-based nanophotocatalysts.
Phosphorene (BP), a newly emerging two-dimensional (2D) layered black phosphorus [1, 2], has attracted a surge of interest for energy storage, catalysis, and sensor application  due to the extraordinary properties such as remarkable high hole mobility (10,000 cm2 V−1 s−1)  and widely tunable band structures (0.3–2 eV) [5, 6]. However, BP easily absorbs the small molecules including external water and oxygen in ambient conditions, resulting in its instability, which hinders its practical applications [7,8,9,10]. Recent works have demonstrated that the formation of van der Waals (vdW) heterostructures between BP and other nanomaterials can extremely improve its stability because other nanomaterials grown on the surface of BP as a contact inhibitor could prevent it from reacting with the small molecules from ambient conditions [11,12,13,14,15,16,17]. Chen et al. reported that the electrical performance of BN-BP heterostructure shows no degradation after exposure to ambient conditions for a whole week . Yuan et al. found that the BP/MoS2 composites exhibit high stability and excellent photocatalytic activity (62 times higher rate of hydrogen generation than that of bare BP under visible-light irradiation) .
The low-dimensional carbon nanomaterials such as graphene, carbon nanotubes (CNTs), and fullerene have been widely applied due to their unique physical and chemical properties [18,19,20]. Various carbon nanomaterials/BP composites have been designed and synthesized owing to high stability and excellent optic-electronic properties as compared to isolated phosphorene for meeting distinct electronic and optoelectronic application [21,22,23,24,25]. BP is stabilized by graphene as a thin passivation layer at least several months . BP/g-C3N4 hybrids show excellent and stable photocatalytic activities for H2 evolution and rapid degradation of RhB under visible light . In particular, Chen et al. directly prepared CNT/BP 1D/2D heterostructures from red phosphorus into BP in the highly dispersed CNT matrix by a thermal-vaporization transformation method, exhibiting high stability and efficient oxygen evolution reaction (OER) activity comparable to that of commercial RuO2 electrocatalysts because of their unique geometrical and electronic characteristics . BP sheets incorporated with CNT are produced by adding N-methyl-2-pyrrolidone–based BP solution into the aqueous single-walled CNT dispersion and have the improved charge transfer properties and suppressed recombination rate, and the high stability in ambient conditions .
To exploit the application potential of CNT/BP heterojunction as photocatalysts, the electronic structures and interfacial interaction is systematically explored by large-scale density functional theory (DFT) computations. Single-walled zigzag CNTs with different diameters varied in a wide range (0.3~20.0 nm) are employed to construct the BP/CNT heterostructures, because the electron structure of CNTs changes with the diameter  and will therefore influence the photoelectric properties of CNT/BP nanocomposites. More importantly, the (5,0), (7,0), (8,0), and (10,0) CNTs are semiconductors, while the (3,0), (6,0), and (9,0) CNT are metallic in nature. Therefore, the investigated CNT/BP composites are representative to elucidate the exact mechanisms of excellent photoelectric activity because the carbon nanotubes used in the experiments are usually a mixture of metallic and semiconducting tubes in nature. Here, we explicitly show that the interfacial interaction in the CNT/BP hybrid is a weak vdW interaction and related to tube diameter of CNTs. All the CNT/BP hybrids have a small band gap (< 0.8 eV) and strong optical absorption compared with that of individual BP and CNT. A diameter-dependent type I or II heterojunction in CNT/BP hybrids is observed. CNTs can effectively improve the stability of BP. These findings indicate that CNT/BP hybrids should be a good candidate as a photocatalyst, which can contribute in developing highly efficient phosphorene-based or CNT-based nanophotocatalysts.
To construct CNT/BP heterostructures, the (1 × 1 × 1) CNTs are respectively used to represent typical ∼ 0.43 nm CNTs. The calculated supercells are composed of a (1 × 5) monolayer BP (containing 20 P atoms) and different carbon tubes with length of 4.26 Å in its axial direction. This only causes minor axial strain, leading to a 1.3% lattice mismatch. The vacuum depth is as large as 15 Å for all the hybrids to avoid artificial interaction in a supercell (4.4 × 16.5 × 28 Å3). All of the theoretical calculations are performed using the density functional theory (DFT) method implemented in the plane wave basis CASTEP code . The Perdew−Burke−Ernzerh (PBE) type of generalized gradient approximation (GGA) exchange correlation functional  is chosen. Although the PBE functional may underestimate the band gaps, the calculated features and tendencies in the BP/CNT hybrids should still be qualitatively reliable . The interlayer van der Waals (vdW) interaction needs to be considered by employing a semi-empirical correction scheme of Grimme’s DFT-D2 method . A Morkhost-Pack mesh of k points, 5 × 8 × 1 points, is used, to sample the two-dimensional Brillouin zone for geometry optimization and for calculating the density of states (DOSs). The cutoff energy for plane waves is chosen to be 400 eV, total energy, and all forces on atoms converge to less than 10−6 eV and 0.01 eV/Å, respectively.
Results and Discussion
Geometric Structure and Formation Energy
Experimental evidences exhibit that whether the CNT is the metallic or semiconducting is closely associated with their tube diameter (D) and the helicity of the arrangement of graphitic rings in their walls . The controlling diameter in the fabrication of single-walled carbon nanotube (SWNT) arrays is a crucial aspect for determining their properties and their integration into practical devices [35,36,37]. To clarify the effect of tube diameter on the interface interaction in the CNT/BP heterostructures, seven zigzag single-walled CNTs with different diameters ranging from 2.35 to 7.83 Å (see Table 1) are chosen.
Figure 1 shows the side and top view of the optimized geometric structures for four representative CNT/BP heterostructures: (5,0) CNT/BP, (6,0) CNT/BP, (9,0) CNT/BP, and (10,0) CNT-BP hybrids, respectively. For the optimized CNT-BP hybrids, the equilibrium distances between the nanotube wall and the top P atom of monolayer BP are 2.80~2.93 Å (see Table 1), which is about comparable to those between monolayer BP (or CNT) and other materials (3.49 Å for graphene/BP , 3.46 Å for BN/BP , 2.15–3.60 Å for BP/monolayer TMD , 2.78–3.03 Å for MoS2/CNT , 2.73–2.86 Å for CNT/Ag3PO4 ). Such large equilibrium distance shows that the CNTs interact with monolayer BP through a weak vdWs force. After optimization, the CNTs and monolayer BP in the hybrids are nearly unchanged, further indicating that the CNT-BP interaction is indeed vdW rather than covalent, in consistency with the others’ results .
The stability of the CNT/BP hybrids can be evaluated according to their absorption energy:
where Ecomb, ECNT, and EBP is the total energy of the relaxed CNT/BP, pure CNT, and monolayer BP, respectively. In accordance with the above definition, the negative Ef implies that the interface is stable. All the formation energy for CNT/BP hybrids are negative, almost monotone decreasing from − 0.5930 to − 1.6965 eV with increasing the tube diameter (as seen in Table 1). As a result, it is easy to conclude that these hybrids have the high thermodynamic stability and a rather strong interaction between CNT and monolayer BP. However, it is hard to distinguish that the interface coupling between the (10,0) CNT and BP is stronger than that for (3,0) CNT/BP on the basis of their formation energy. In fact, the CNT(9,0)/BP and CNT(10,0)/BP hybrids with lower formation energy would be more easily formed due to their larger contact area of the CNT with BP.
Band Structure and Density of States
In order to explore the effect of CNT on the electronic properties of monolayer BP, the band structures and density of states (DOSs) for bulk BP, monolayer BP, pure CNT, and CNT/BP hybrids are calculated (Figs. 2 and 3; Table 1). Figure 2e and f show that the valence band (VB) maximum and the conduction band (CB) minimum in our calculated bulk BP and monolayer BP are located at the G point of the Brillouin zone, which is a confirmation of the clear direct band gap (Eg) semiconductor with 0.3 and 0.94 eV, consistent with previous research results  and their DOSs (Fig. 3d, d*). In addition, it can also be seen that the top of VB is more dispersive than the bottom of CB for BP and the hybrids, suggesting that the photogenerated holes possess smaller effective masses. The electronic characteristics in BP and the CNT/BP hybrids can promote the separation of electron–hole pairs during the reaction process and result in good photocatalytic activity.
Figure 3 shows the density of states (DOSs) of individual CNT, BP, and their hybrids. As seen in part c* of Fig. 3, (9, 0) CNT is metallic, which agrees well with the previous studies . After attentively observing Fig. 3, it is easy to conclude that each component of the combined DOSs changes very little relative to those of individuals in the CNT/BP hybrids, basically maintaining the nature of their respective DOSs as isolated individuals, which is indicative of the existence of indeed weak vdW interaction at the CNT-BP interface and corresponds to large equilibrium distance between the CNT and monolayer BP in the hybrids (2.80〜2.93 Å).
The calculated band gaps of the semiconducting (5, 0), (7, 0), (8, 0), and (10, 0) CNT-BP hybrids are 0.190, 0.315, 0.375, and 0.863 eV, respectively, as listed in Table 1. Particularly, as the metallic (3,0), (6,0), and (9,0)CNTs are coupled to BP, all the metallic CNTs open a band gap due to the stress effect, similar to the previous work in CNT/MoS2 hybrids . And even more interesting, the variation of band gap in the CNT/BP hybrids is in a monotonic increase with tube diameter, indicating that the influence of CNT on the electronic properties of the BP is related with the tube diameter. Therefore, it is an effective approach for the CNT/BP hybrids to tune their band gap by CNT tube diameter. In the CNT/BP hybrids, all band gaps calculated are small (< 0.9 eV, as listed in Table 1). Such band gaps have the CNT/BP hybrids absorb most of the sunlight that more photogenerated electrons are excited from the valence band (VB) to the conduction band (CB) of the heterostructures, enhancing photocatalytic performance of CNT/BP compared with monolayer BP.
Although the small band gap to capture visible light which contributes about 50% solar radiation energy plays an important role in the photocatalytic effect, it seems to be not a unique role. Actually, the effective separation of photogenerated charge carriers is also an important factor for improving photocatalytic performance . As demonstrated clearly in Fig. 3, each component of the combined DOSs in the CNT/BP hybrids is mutually staggered near the Fermi level. Hence, such small band gaps in CNT/BP hybrids can be understood in a simple mechanism that the C 2p states of CNT appear in the gap of monolayer BP. Also, it is found that the near-gap electronic structure of CNT/BP hybrid varies with tube diameter. As the small CNTs (such as (5, 0) and (6, 0) tubes) are combined with monolayer BP, their energy levels are embedded in the band gap of monolayer BP (Figs. 3a, b), which can be more clearly seen from the electron density distributions of the highest occupied and lowest unoccupied levels (HOL and LUL), as demonstrated in Fig. 4. The highest occupied level (HOL) is composed of C 2p states and a small P states in CNT(6, 0)/BP, even only formed by C 2p states in CNT(5, 0)/BP, where their lowest unoccupied levels (LUL) are all composed of the C 2p orbits mixing a small P state. As a result, the CNT(5, 0)/BP and CNT(6, 0)/BP exhibited type I heterojunctions . For practical purpose as photocatalysis, such band alignment is not beneficial for the separation of photogenerated electron−hole pairs but recombine readily on CNT. Consequently, the CNT might play a part of recombination centers and reduce the photocatalytic activities of CNT/BP hybrids. On the contrary, as large diameter (9, 0) CNTs are coupled to monolayer BP, their energy levels are staggered (Fig. 3c), forming a type II heterojunctions. This is also further confirmed from the two right-most columns in Fig. 4: LUL is C states and HOL is P states.
In photocatalysis, such a type II band alignment is believed to have a remarkable infIuence on the efficient separation of the photogenerated electron–hole pairs. Under light irradiation, the electrons can be directly excited from monolayer BP to CNTs and consequently result in the efficient charge separation between the two constituents. In addition, forming a type II heterostructure is an effective approach to extend the photoresponse region. As a result, a large diameter of (9, 0) CNTs is a sensitizer for monolayer BP. These results have revealed that coupling large diameter of CNTs on the monolayer BP should be a well-chosen road for achieving high photoactivity.
Charge Density Difference and Mechanism Analysis
All changes of the DOSs mentioned above are originated from interfacial interaction between the involved constituents, and the interfacial interaction is highly correlated with charge transfer in heterojunctions. Actually, it can be understood in a simple mechanism based on the extent of charge transfer at the interface: the stronger coupling and the more charge transfer. Based on 3D charge density difference, the charge transfer and redistribution at the interface in these hybrids can be evaluated (as shown in Fig. 5) by the following relationship:
where ρCNT/BP, ρBP, and ρCNT denote, respectively, the charge densities of the hybrids, monolayer BP, and CNT in the same configuration. In Fig. 5, the blue and yellow represent charge accumulation and depletion, respectively. Obviously, the charge redistribution is visible due to the interaction in the CNT/BP hybrid, involving all C atoms in CNT, the top p atom in BP (Fig. 5a1–b2). Moreover, a strong charge depletion (blue part in Fig. 5), is found mainly from top p atoms in BP. This indicates that CNTs are more attractive to electrons, which is helpful for enhancing the stability of monolayer BP photocatalyst.
The quantitative result of charge transfer and redistribution is plotted in Figs. 5d1 and d2 by the planar averaged charge density difference along the direction perpendicular to the monolayer BP. The horizontal dashed lines are the positions of both the bottom layer of the CNT and the top p atom of monolayer BP. The positive (negative) values indicate electron accumulation (depletion). The largest efficient electron depletion localized above the p atoms of monolayer BP is about − 1.29 × 10−2 e/Å3 in the CNT/BP hybrids, while the largest efficient electron accumulation localized at the lowest layer C atoms is about 1.41 × 10−2, 1.63 × 10−2, 1.84 × 10−2, and 1.96 × 10−2 e/Å3 in the CNT(5,0)/BP, CNT(6,0)/BP, CNT(9,0)/BP, and CNT(10,0)/BP hybrids. This demonstrates that the interfacial interaction between the CNT and monolayer BP gets stronger with increasing diameter of the CNT, which may be caused by the increases of the contact area between the CNT and the BP with increasing diameter of the CNT.
The quantitatively charge variation at the interface can also be figured out by a Mulliken population analysis of the plane wave pseudopotential calculations on the CNT, monolayer BP, and CNT/BP hybrids. Figure 6 shows the results of the Mulliken charge on C and P atoms in the CNT/BP hybrids, in which several typical values are presented. The top p atom of monolayer BP has a Mulliken charge of 0.01. The charge variation declares that the top-most P atoms of the CNT/BP hybrids would lose more electrons than those in the isolated monolayer BP (a Mulliken charge of approaching zero in pure monolayer BP).
Although the C atoms in the CNT have a Mulliken charge of approaching zero, those C atoms in the CNT/BP hybrids have different Mulliken charges because the interfacial interaction is varied. Figure 6 shows that the bottom layer C atom near monolayer BP has a Mulliken charge of − 0.01 and − 0.02 in the CNT(5,0)/BP and CNT(6,0)/BP hybrids, further depicting the interfacial interaction improvement with increasing nanotube diameter, corresponding to an increasing contact area in the CNT/BP hybrids.
The effective net charge from one constituent to another in these composites can be studied by the Bader method, as listed in Table 1. The calculated Bader charge reveals that some charge is transferred from BP to CNTs, thus leading to hole doping for the BP, which is in line with the planar averaged charge density difference. Interestingly, the amount of charge transferred in these hybrids depends upon the tube diameter. When the tube diameter becomes big (2.35–7.8 Å), the electrons transferred from BP to CNT in the CNT hybrids (Table 1) also increases (0.004–0.142), in agreement with the fact that the former has the increasing interfacial contact area in the CNT/BP hybrids.
The interfacial charge transfer will result in the variation of electrostatic potential distribution at the interface in the hybrids. Figure 5c1 and c2 display specific position in the z-direction dependence of the profile of the planar averaged self-consistent electrostatic potential for the CNT/BP hybrids. At the interface, a potential difference of ~ 0.39 eV between CNT and monolayer BP can be observed for CNT(9,0)/BP and CNT(10,0)/BP, while the average electrostatic potential difference is 0.37 eV for CNT(5,0)/BP and CNT(6,0)/BP, where there is a minor change of potential at the interface. Under light irradiation, the built-in potential at the CNT-BP interface can improve the separation and migration of photogenerated carriers in the hybrids, which would greatly enhance the photocatalytic activity and stability of the CNT/BP photocatalyst.
To assess the optical properties of monolayer BP and CNT/BP hybrids, their imaginary parts ɛ2 of the dielectric function are calculated from the momentum matrix elements between the occupied and unoccupied wave functions based on the Fermi golden rule within the dipole approximation by the following equation:
where ɛ2, ħɷ, p, (| kn〉), and f(kn) are the imaginary part of the dielectric function, the energy of the incident photon, the momentum operator r(ħ/i)(∂/∂x), a crystal wave function, and Fermi function, respectively. The real part ε1(ω) of the dielectric function can be obtained from imaginary part according to Kramers–Kronig relationship. The optical absorption coefficient I(ω) can be evaluated using the following formula:
The relations above are the theoretical basis of band structure and optical properties to explain the mechanism of absorption spectral caused by electronic transition between different energy levels. Figure 7 presents the calculated UV-vis absorption spectra of monolayer BP and CNT/BP hybrids. The absorption edge of monolayer BP is located next to 0.93 eV corresponding to its intrinsic transition from the 3s to the 3p orbitals. The optical absorption edge of the CNT/BP hybrid shifts towards the longer wavelength than that of pure monolayer BP due to their decreased band gaps (see Fig. 7), as a result of the electron transition from the C 2p to P 3P states, or C 2p to C 2p states.
The strong absorption intensity is one of the most important factors for a superior photocatalyst. Compared with that of monolayer BP as illustrated in Fig. 7, the optical absorption of CNT/BP hybrids can be improved significantly in the visible-light region. It is understandable to think that the weak optical absorption of pure BP in the vis-light region is ascribed to the small values of s−p matrix elements in Eq. 3 due to the very low 3p states in the CB bottom. For the CNT/BP hybrids, C 2p- and P 3p-hybridized orbitals are predominant components at the lower part of CB and VB top (Fig. 3). The large states near the band gap of these CNT/BP hybrids correspond to the big values of s−p and p−p matrix elements in Eq. 3. Therefore, the light absorption of these CNT/BP hybrids is enhanced in the visible-light region (Fig. 7).
For the CNT/BP hybrids, the origins of the improved photocatalytic activity and stability are as follows. Firstly, the C 2p states of CNTs embedded into the band gap of BP (Fig. 3) give rise to more bound electrons taking part in the interband transitions, which not only extends the absorption range but also increases the absorption intensity compared to their individuals. Secondly, experimental results show that the BP/CNTs have a low equivalent resistance, 13 times lower than that of BP . The observed excellent electrocatalytic activity and stability of BP-CNTs is much higher than that of BP, which has been attributed to much lower charge transfer resistance of BP/CNTs compared with that of BP . In the CNT/BP hybrids, CNT networks with a large surface area and high conductivity play a key role of fast conductive bridge and can greatly improve the electrical conductivity of the BP catalyst. Therefore, the photogenerated charges can be shuttled freely along the conducting network of the CNT bundle under vis-light irradiation, and the photoexcited charge carriers can be effectively separated and transferred, resulting in a low carrier recombination rate and high photocatalytic activity. More importantly for the CNT(9,0)/BP hybrids, forming a type-II heterojunction band alignment (Fig. 4) makes the photoexcited electrons and holes move to different sides of heterojunction and subsequently result in an efficiently spatial separation of electron–hole pairs on before recombination . Furthermore, some neutral C atoms are charged due to charge transfer in CNTs, which will become active sites from being initially catalytically inert, making the CNTs to be a highly active co-catalyst in these hybrids. Besides, the number of active sites increased significantly due to the loss of electrons during the photocatalytic process. The synergistic effects of the above factors can result in enhanced vis-light photocatalytic performance of the CNT/BP hybrids. Based on the above analysis, coupling CNT on the BP semiconductor would improve the photocatalytic activity of BP.
In summary, we have investigated the potential applications of the CNT/BP composites in photocatalysis by analyzing the electronic and optical properties under the framework of DFT. Our results show that the CNT/BP hybrids have small band gap (< 0.8 eV), resulting into their strong absorption in not only vis-light region but also near-infrared spectral regions. More importantly, a type II heterojunction can effectively separate the photoexcited charge carriers in CNT(9,0)/BP hybrid and can facilitate the separation of photoexcited electrons and holes. Thus, it is reasonable to conclude that CNT/BP hybrids would be a good candidate as a photocatalyst, which can contribute to developing highly efficient phosphorene-based or CNT-based nanophotocatalysts.
Availability of Data and Materials
The datasets generated during and/or analyzed during the current study are available from the corresponding author on request.
Density functional theory
van der Waals
Oxygen evolution reaction
Generalized gradient approximation
Density of states
Highest occupied levels
Lowest unoccupied levels.
Reich ES (2014) Phosphorene excites materials scientists. Nature 506:19–19
Wang C, He QY, Halim U, Liu YY, Zhu EB, Lin ZY, Xiao H, DuanX D, Feng ZY, Cheng R, Weiss NO, Ye GJ, Huang YC, Wu H, Cheng HC, Shakir I, Liao L, Chen XH, Goddard WA, Huang Y, Duan XF (2018) Monolayer atomic crystal molecular superlattices. Nature 555:231–236
Liu H, Hu K, Yan D, Chen R, Zou Y, Liu H, Wang S (2018) Recent Advances on Black Phosphorus for Energy Storage, Catalysis, and Sensor Applications. Adv. Mater 30:1800295
Qiao JS, Kong XH, Hu ZX, Yang F, Ji W (2014) High-mobility transport anisotropy and linear dichroism in few-layer black phosphorus Nat. Commun 5:1–7
Kim J, Baik SS, Ryu SH, Sohn Y, Park S, Park BG, Denlinger J, Yi Y, Choi HJ, Kim KS (2015) Observation of tunable band gap and anisotropic Dirac semimetal state in black phosphorus. Science 349:723–726
Wang XM, Jones AM, Seyler KL, Tran V, Jia YC, Zhao H, Wang H, Yang L, Xu XD, Xia FN (2015) Highly anisotropic and robust excitons in monolayer black phosphorus. Nat Nanotechnol 10:517–521
Wu S, He F, Xie GX, Bian ZL, Luo JB, Wen SZ (2018) Black phosphorus: degradation favors lubrication. Nano Lett 18:5618–5627
Island JO, Steele GA, van der Zant HSJ, Castellanos-Gomez A (2015) Environmental instability of few-layer black phosphorus. 2D Materials 2:011002
Pei JJ, Gai X, Yang J, Wang XB, Yu ZF, Choi DY, Luther-Davies B, Lu YR (2016) Producing air-stable monolayers of phosphorene and their defect engineering. Nat Commun 7:1–8
Cai YQ, Ke QQ, Zhang G, Zhane YW (2015) Energetics, charge transfer, and magnetism of small molecules physisorbed on phosphorene. J Phys Chem C 119:3102–3110
Chen XL, Wu YY, Wu ZF, Han Y, Xu SG, Wang L, Ye WG, Han TY, He YH, Cai Y, Wang N (2015) High-quality sandwiched black phosphorus heterostructure and its quantum oscillations. Nat. Commun 6:1–6
Yuan YJ, Wang P, Li ZJ, Wu YZ, Bai WF, Su YB, Guan J, Wu ST, Zhong JS, Yu ZT, Zou ZG (2019) The role of bandgap and interface in enhancing photocatalytic H2 generation activity of 2D-2D black phosphorus/MoS2 photocatalyst. Appl. Catal. B-Environ. 42:1–8
Yuan JT, Najmaei S, Zhang ZH, Zhang J, Lei SD, Ajayan PM, Yakobson BI, Lou J (2015) Photoluminescence quenching and charge transfer in artificial heterostacks of monolayer transition metal dichalcogenides and few-layer black phosphorus. ACS Nano 9:555–563
Dai J, Zeng XC (2014) Bilayer phosphorene: effect of stacking order on bandgap and its potential applications in thin-film solar cells. J. Phys. Chem. Lett. 5:1289–1293
Koda DS, Bechstedt F, Marques M, Teles LK (2017) Tuning electronic properties and band alignments of phosphorene combined with MoSe2 and WSe2. J. Phys. Chem. C 121:3862–3869
Hu L, Yuan J, Ren Y, Wang Y, Yang JQ, Zhou Y, Zeng YJ, Han ST, Ruan SC (2018) Phosphorene/ZnO Nano-Heterojunctions for broadband photonic nonvolatile memory applications. Adv. Mater. 30:9
Niu XH, Li YH, Zhang YH, Zheng QJ, Zhao J, Wang JL (2019) Highly efficient photogenerated electron transfer at a black phosphorus/indium selenide heterostructure interface from ultrafast dynamics. J. Mater. Chem. C 7:1864–1870
Su DS, Perathoner S, Centi G (2013) Nanocarbons for the development of advanced catalysts. Chem. Rev. 113:5782–5816
Zeng F, Huang WQ, Xiao JH, Li YY, Peng W, Hu WY, Li K, Huang GF (2019) Isotype Heterojunction g-C3N4/g-C3N4 Nanosheets as 2D support to highly dispersed 0D metal oxide nanoparticles: generalized self-assembly and its high photocatalytic activity. J. Phys. D-Appl. Phys. 52:025501
Qiao Q, Yang K, Ma LL, Huang WQ, Zhou BX, Pan AL, Hu WY, Fan XX, Huang GF (2018) Facile in situ construction of mediator-free direct Z-Scheme g-C3N4/CeO2 heterojunctions with highly efficient photocatalytic activity. J. Phys. D-Appl. Phys. 51:275302
Kim J, Baek SK, Kim KS, Chang YJ, Choi EJ (2016) Long-term stability study of graphene-passivated black phosphorus under air exposure. Curr. Appl. Phys. 16:165–169
Cai YQ, Zhang G, Zhang YW (2015) Electronic properties of phosphorene/graphene and phosphorene/hexagonal boron nitride heterostructures. J. Phys. Chem. C 119:13929–13936
Rajbanshi B, Kar M, Sarkar P, Sarkar P (2017) Phosphorene quantum dot-fullerene nanocomposites for solar energy conversion: an unexplored inorganic-organic nanohybrid with novel photovoltaic properties. Chem. Phys. Lett. 685:16–22
Ran JR, Guo WW, Wang HL, Zhu BC, Yu JG, Qiao SZ (2018) Metal-Free 2D/2D Phosphorene/g-C3N4 Van Der Waals heterojunction for highly enhanced visible-light photocatalytic H2 production. Adv. Mater. 30:1800295
Zhu MS, Kim S, Mao L, Fujitsuka M, Zhang JY, Wang XC, Majima T (2017) Metal-free photocatalyst for H2 evolution in visible to near-infrared region: black phosphorus/graphitic carbon nitride. J. Am. Chem. Soc. 139:13234–13242
Clark N, Nguyen L, Hamer MJ, Schedin F, Lewis EA, Prestat E, Garner A, Cao Y, Zhu MJ, Kashtiban R, Sloan J, Kepaptsoglou D, Gorbachev RV, Haigh SJ (2018) Scalable patterning of encapsulated black phosphorus. Nano Lett. 18:5373–5381
Jiang Q, Xu L, Chen N, Zhang H, Dai L, Wang S (2016) Facile synthesis of black phosphorus: an efficient electrocatalyst for the oxygen evolving reaction. Angew.Chem.Int.Ed. 55:13849–13853
Bat-Erdene M, Batmunkh M, Tawfik SA, Fronzi M, Ford MJ, Shearer CJ, Yu LP, Dadkhah M, Gascooke JR, Gibson CT, Shapter JG (2017) Efficiency enhancement of single-walled carbon nanotube-silicon heterojunction solar cells using microwave-exfoliated few-layer black phosphorus. Adv. Funct. Mater. 27:1704488
Matsuda Y, Tahir-Kheli J, Goddard WA (2010) Definitive band gaps for single-wall carbon nanotubes. J. Phys. Chem. Lett. 1:2946–2950
Zan WY, Geng W, Liu HX, Yao XJ (2015) Influence of interface structures on the properties of molybdenum disulfide/graphene composites: a density functional theory study. J. Alloy. Compd. 649:961–967
Perdew JP, Burke K, Ernzerhof M (1996) Generalized gradient approximation made simple. Phys. Rev. Lett. 77:3865–3868
Tian XQ, Wang XR, Wei YD, Liu L, Gong ZR, Gu J, Du Y, Yakobson BI (2017) Highly tunable electronic structures of phosphorene/carbon nanotube heterostructures through external electric field and atomic intercalation. Nano Lett. 17:7995–8004
Grimme S (2006) Semiempirical GGA-type density functional constructed with a long-range dispersion correction. J. Comput. Chem. 27:1787–1799
Odom TW, Jin-Lin H, Kim P, Lieber CM (1998) Atomic structure and electronic properties of single-walled carbon nanotubes. Nature 391:62–64
Leonard F, Talin AA (2006) Size-dependent effects on electrical contacts to nanotubes and nanowires. Phys. Rev. Lett. 97:026804
Chen ZH, Appenzeller J, Knoch J, Lin YM, Avouris P (2005) The role of metal-nanotube contact in the performance of carbon nanotube field-effect transistors. Nano Lett. 5:1497–1502
Kim W, Javey A, Tu R, Cao J, Wang Q, Dai H (2005) Electrical contacts to carbon nanotubes down to 1 nm in diameter. Appl. Phys. Lett. 87:173101
You BQ, Wang XC, Zheng ZD, Mi WB (2016) Black phosphorene/monolayer transition-metal dichalcogenides as two dimensional van der Waals heterostructures: a first-principles study. Phys. Chem. Chem. Phys. 18:7381–7388
Zhang ZG, Huang W-Q, Xie Z, Hu W, Peng P, Huang G-F (2017) Noncovalent functionalization of monolayer MoS2 with carbon nanotubes: tuning electronic structure and photocatalytic activity. J. Phys. Chem. C. 121:21921–21929
Zhang ZG, Huang W-Q, Xie Z, Hu W, Peng P, Huang G-F (2017) Simultaneous covalent and noncovalent carbon nanotube/Ag3PO4 Hybrids: new insights into the origin of enhanced visible light photocatalytic performance. Phys. Chem. Chem. Phys. 19:7955–7963
Du YL, Ouyang CY, Shi SQ, Lei MS (2010) Ab initio studies on atomic and electronic structures of black phosphorus. J. Appl. Phys. 107:093718
Li HJ, Zhou Y, Tu WG, Ye JH, Zou ZG (2015) State-of-the-art progress in diverse heterostructured photocatalysts toward promoting photocatalytic performance Ab initio studies on atomic and electronic structures of black phosphorus. Adv Funct Mater. 25:998–1013
Yang BC, Hao CX, Wen FS, Wang BC, Mu CP, Xiang JY, Li L, Xu B, Zhao ZS, Liu ZY, Tian YJ (2017) ACS Appl Mater Interfaces. 9:44478–44484
This work was supported by the National Natural Science Foundation of China (Grant Nos. 51772085, U1830138, and U1530151).
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Zhang, Z., Cheng, M., Chen, Q. et al. Monolayer Phosphorene–Carbon Nanotube Heterostructures for Photocatalysis: Analysis by Density Functional Theory. Nanoscale Res Lett 14, 233 (2019). https://doi.org/10.1186/s11671-019-3066-z
- Carbon nanotube
- Electronic structure
- Photocatalytic performance
- Interfacial interaction
- First-principle calculations